AN INVESTIGATION OF DEFECTS ON BUTT JOINT OF DIFFERENT WELDING TECHNIQUE USING ULTRASONIC
MOHD AUDI AIZAT BIN MOHD ZIM
This report is represented as part of the requirements of Bachelor of Mechanical Engineering (Structure-Material)
Faculty of Mechanical Engineering University Teknikal Malaysia Melaka
“I hereby declare that I have read this thesis and in my opinion this report is sufficient in terms of scope and quality for the award of the degree of
Bachelor of Mechanical Engineering (Structure and Material)”
“I hereby declare that the work in this report is my own except for summaries and quotations which have been duly acknowledged.”
Signature : ... Author : MOHD AUDI AIZAT BIN MOHD ZIM
Alhamdulillah, praise to Allah the Almighty because only by His will, I had finally finished preparing this PSM thesis for this semester Final Year Project.I would like to take this opportunity to give my appreciation to Puan Anita Akmar Bte Kamarolzaman for her guidance, support, advices, and her precious time during the course of my project. Moreover, I also would like to thank Dr Thiru in taking effort to read this thesis and give advices thoughts of knowledge to improve my report.
Fokus projek ini adalah untuk mengesan kedudukan kecacatan atau ketaksinambungan di dalam sendi yang dikimpal atas sampel spesimen besi dua fasa dengan menggunakan kaedah ujian tanpa musnah (NDT) iaitu Ujian Ultrasonik (UT). Dalam projek ini, 4 keping plat besi yang telah dirawat di sambung di penghujung plat dengan menggunakn kaedah proses kimpalan arka (SMAW) dan gabungan kimpalan gas lengai tungsten (TIG-C) menjadi 2 spesimen. Kedua-dua spesimen ditandakan sebagai plat C1 dan C2. Proses kimpalan dilakukan oleh pengimpal yang berpengalaman untuk mendapatkan sekeping hasil kimpal yang baik. Pemeriksaan hasil kimpal dengan menggunakan ujian ultrasonik berlaku selepas semua proses kimpalan telah selesai. Permulaan proses UT dengan penentukuran siasatan di mana siasatan ditentukur dengan blok tentukuran V1 dan V2 sebelum ke pemeriksaan plat. Terdapat tiga jenis probe sudut yang terdiri daripada 45 ˚, 60 ˚, 70 ˚, tetapi untuk projek ini 70o prob sudut digunakan untuk
2.2.2 Medium Carbon Steel 5
2.2.4 Heat Treatment Process 11
220.127.116.11 Quenching 11
2.3 Dual Phase Steel 12
2.4 Welding 13
2.4.1. Tungsten Inert Gas Welding (TIG) 13 18.104.22.168 Combined Tungsten Inert Gas (TIG-C) 13 2.4.2 Shielded Metal Arc Welding (SMAW) 14 22.214.171.124 Type of Welded Joint 15
126.96.36.199.1 Butt Joint 16
2.5 Non Destructive Testing 17 2.5.1 Ultrasonic Testing (UT) 17 188.8.131.52 Characteristic of Ultrasound 18 184.108.40.206.1 Wave Propagation 18
220.127.116.11 Ultrasonic Beam 22
18.104.22.168 Beam Spread 24
22.214.171.124 Attenuation of Ultrasonic Beam 25 126.96.36.199.1 Scattering of Ultrasonic Waves 25 188.8.131.52.2 Absorption of Ultrasonic Waves 26 184.108.40.206.3 Loss Due To Coupling 26
220.127.116.11 Instrumentation 26
18.104.22.168.3 Couplant 30
22.214.171.124.4 Ultrasonic Flaw Detector (UTFD) 30 2.5.2 Radiography Testing (RT) 31
3.3.4 Heat Treatment Process 35
3.3.5 Quenching Process 36
3.3.6 Welding Process 36
126.96.36.199 Type of joint 37
3.4 Non Destructive Testing (NDT) 37 3.4.1 Determination of Angle Probe 39 3.4.2 Time Base Calibration 40 3.4.3 Determination of Probe Index 41 3.4.4 Distance Amplitude Correction (DAC) Curve 41
3.4.5 Inspection 42
188.8.131.52 ASME V Article 4 42
3.4.6 Evaluation 43
CHAPTER 4 RESULT AND DISCUSSION 46
4.1 Introduction 46
4.2 Calibration Process 47
4.2.1 Time Base Calibration 47 4.2.2 Determination of Probe Index 48 4.2.3 Distance Amplitude Correction (DAC) Curve 48
4.3 Result and Discussion 49
4.3.1 C1 Plate 49
184.108.40.206. Discussion 52
220.127.116.11.1. Lack of Sidewall Fusion 52 18.104.22.168.2. Tungsten Inclusion 53
4.3.2 C2 Plate 54
22.214.171.124. Discussion 57
126.96.36.199.1. Lack of Fusion 57
188.8.131.52.2. Porosity 58
CHAPTER 5 CONCLUSION & RECOMMENDATION 59
5.1. Conclusion 59
5.2. Recommendation 60
LIST OF TABLES
NO. TITLE PAGE
LIST OF FIGURES
NO. TITLE PAGE
2.1 The iron-iron carbide phase diagram. 6
2.2 Alpha Ferrite Microstructure. 7
2.3 Austenite Microstructure 8
2.4 Pearlite Microstructure 9
2.5 Martensite Microstructure 10
2.6 The TTT diagram for AISI 1080 steel (0.79%C, 0.76%Mn) austenitised at 900°C 11 2.7 Presence of Martensite in Dual Phase Steel. 12 2.8 TIG Welding Technique Schematic Diagram 13 2.9 Shielded Metal Arc Welding Schematic Diagram 14
2.10 Welding Butt Joint 16
2.11 V-Groove Butt Joint 16
2.12 Bevel Groove Butt Joint 17
2.13 Analogy of Sound Wave Propagate in a Solid Region 18
2.14 Analogy of Longitudinal Waves 19
2.15 Analogy of Shear Waves 20
2.17 Analogy of Lamb Waves 21
2.18 Ultrasonic Beam Region 22
2.19 Construction Waves Surfaces from Elementary Waves 23 2.20 Distribution of Intensity along the Axial Distance 23
2.21 Beam Spread from a Transducer 24
2.22 Attenuation Losses during Transmission 25
2.23 Normal Probe Diagram 27
2.24 Angle Probe Diagram 28
2.25 Twin Crystal Diagram 29
2.26 V1 Calibration Block 29
2.27 V2 Calibration Block 30
2.28 Schematic Diagram for Radiographic Testing 31
3.1 Flow Chart 33
3.2 Specimen Dimension 34
3.3 Beveling of 30o degree for one end of specimen 35
3.4 Butt joint Weldment 37
3.5 UTFD Flow Chart 38
3.6 70o Angle Probe 39
3.10 Determination of Probe Index on V1 Calibration Block 41
3.11 Schematic Diagram to Measure the Defect. 43
3.12 Radiographic Testing Parameter. 44
3.13 Radiographic Testing in Progress. 45 4.1 Schematic Diagram to Measure the Defect 46
4.2 Completed Time Base Calibration 47
4.3 Maximum Amplitude at High Intensity of Sound Wave. 48 4.4 Developed DAC Curve for 70o Angle Probe. 48
4.5 Localize Defect on Plate C1 49
4.6 Lack of Side Wall Fusion Defect Echo 50
4.7 Tungsten Inclusion Defect Echo 50
4.8 Radiographic Indication on Plate C1 51 4.9 Diagram for Lack of Sidewall Fusion 52
4.10 Localize Defect in Plate C2 54
4.11 Gas Porous Defect echo Indication 55 4.12 Lack of Fusion Defect Echo Indication 55 4.13 Radiographic Indication on Plate C2 56
4.14 Lack of Fusion 57
Automotive manufacturer nowadays widely used of aluminum as their material to build cars. Due to its lightweight and strong characteristic, aluminum is a suitable replacement for steel in modern cars body frame, comes with expensive price. Therefore, as the alternative, steel has been upgraded to dual phase steel through heat treatment process. Its increase its strength but remains its good features such as good formability, weight, and price.
In body of a car, it involves hundreds of joint from various part of the car body panel. Each body panel is joined by different welding process. Welding process commonly used in automotive industry is combined tungsten inert gas (TIG-C) and shielded metal arc welding (SMAW). Different welding process used in different joint. Therefore, welding codes and specification has been created to guide the welders to choose the proper welding technique to be used in different joints.
Car body frame consist of many part that joined together by welding process. There are spot welding process for critical joints such as main body frame, butt TIG-C and SMAW welding process for butt joint, and some more. Different type of joints required different types of welding process. However, errors occurred during the welding process which leads to some discontinuities, crack, and flaws on the welded part. This can be dangerous since the crack exist on the welded part can distribute to the fracture of the vehicle. Non-destructive method had been used to identify the cracks on different weld joint such as T-joint, butt joint and dissimilar joint.
Dual phase steel has a great potential to be used as the outer body panel in automotive industry due to its high strength and good formability. However, discontinuities developed during the TIG-C and MIG welding process can be considered dangerous and past from the tolerate level. To identify the possible defects and the behavior of the flaws, ultrasonic testing methods will be applied in this project. In accordance to the ASTM standard practice for the ultrasonic testing, this method will be conducted and use to analyze the defect size and types of the butt welded joint.
The objectives of this project are:
1. To produce a dual phase steel by doing a heat treatment on a low carbon steel
3. To compare the result from ultrasonic testing with the X-Ray testing technique.
4. To identify the types of defect found in welded specimen.
2.1. Introduction of Steel.
Steel is a material that generally strong, durable, malleable containing alloying element such as manganese, chromium, nickel and carbon . Steel that has carbon as the alloying element will has either brittle or strong characteristic depends on the carbon content in the steel and also known as carbon steel .
2.2. Type of Steel
There are three types of carbon steel which is low carbon steel, medium carbon steel, and high carbon steel.
2.2.1. High Carbon Steel
2.2.2. Medium Carbon Steel
Medium carbon steel generally has carbon concentration between 0.25 and 0.60 wt% . Different from high carbon steel, medium carbon steel has lowered mechanical properties in term of hardness, strong, brittleness, and some more. However, these mechanical properties of medium carbon steel can be optimizing by doing heat treatment process where the microstructure of the medium carbon steel were changed into martensite microstructure . In order to get high in strength and hardness, medium carbon steel has to sacrifice its ductility and toughness.
Some applications of medium carbon steel is in automotive industry where it use medium carbon steel as body panel in a car. Another example of application in medium carbon steel is railway wheels, railway tracks, gears, and machines part where it require material of high strength and wear resistance.
2.2.3. Low Carbon Steel
In low carbon steel, the carbon contain were less than 0.25 wt% . Low carbon steel microstructure consists of ferrite and pearlite microstructure. The existence of ferrite and pearlite in the low carbon steel gave the low carbon steel an outstanding ductility and toughness . Besides, it also give the low carbon steel the ability of good machinability, weld able and low carbon steel is also less expensive than the two carbon steel. Heat treatment and quenching process of low carbon steel will change the microstructure of the low carbon steel from ferrite and pearlite to ferrite martensite microstructure . The existence of martensite after quenching process, increase the low carbon steel toughness, hardness, and maintain its machinability and ductility features.
184.108.40.206. Iron-iron Carbide Phase Diagram
Figure 2.1 shows the phase diagram for iron-iron carbide. Based on the phase diagram, 727oC is the eutectoid temperature. Beyond this eutectoid temperature line, the microstructure of the iron will change into alpha ferrite and austenite microstructure. The X-axis for the phase diagram represents the percentage of carbon content in the steel. While the Y-axis represents the temperature in degree Celsius (oC) and Fahrenheit (oF). Since in this project we used low carbon steel, therefore the
region that covered by the low carbon when doing a heat treatment is only in the Region A.
Figure 2.1: The iron-iron carbide phase diagram.
220.127.116.11. Ferrite (α-iron)
Alpha ferrite (α iron) is the stable form of iron in a room temperature. Alpha ferrite has the body centered cubic (BCC) crystal structure where a cubic unit cell having atoms positioned at all eight corners and a single atom at the cube center. With the 0.68 packing density, body centered cubic crystal (BCC) structure has a little dislocation movement among the atoms since it has small gap between the atoms. Figure 2.2 shows the microstructure of alpha ferrite under the microscope with the magnifying of 90 times zoom.
Figure 2.2: Alpha Ferrite Microstructure. [Source: “Fundamentals of Materials Science and
18.104.22.168. Austenite (γ-iron)
Gamma phase iron is the other terms for austenite where it is a transformation of the alpha ferrite iron which exists above the critical eutectoid temperature in the iron-carbide phase diagram (Figure 2.1). Based on the Figure 2.3, austenite is a face centered cubic (FCC) crystal structure having a 0.74 packing density allows the atoms to have slip movement among the other atoms since the face centered cubic crystal structure is a close packed lattice structure.
Materials that in this austenite region structure tend to have harder mechanical properties than alpha ferrite. Most of application of austenite iron was used in making of stainless steel to be used in food-service and hospital equipment.
Figure 2.3: Austenite Microstructure [Source: “Fundamentals of Materials Science and
Cementite sometimes called as iron carbide is a combination of iron and carbon in the microstructure of a material. Having Fe3C as its chemical formula,
cementite is a hard and brittle material .
Pearlite is a combination of alpha ferrite and cementite microstructure that commonly occurred in many grades of steels. When a substance is slowly cooled until reach below the eutectoid line of temperature as in Figure 2.1, pearlite microstructure is obtained. For steel that contains higher number of carbon more than 6.7 wt%, it will transform into cementite rather than transform into pearlite microstructure . As shown in Figure 2.4, the black labeled is the pearlite microstructure where, it is the combination of cementite and ferrite microstructure. Furthermore, the white region of the microstructure represent as ferrite microstructure.